LMucko/crystallography-open-database huggingface dataset:
Growth of Sr6 Rh5 O15 single crystals from high-temperature solutions: structure determination using the traditional 3-D and the 4-D superspace group methods and magnetic measurements on oriented single crystals
Stitzer, K.E.; El Abed, A.; Darriet, J.; zur Loye, H.C.; Journal of the American Chemical Society 123 (2001) 8790–8796; doi:

data_4123971
_publ_section_title
;
 Growth of Sr6 Rh5 O15 single crystals from high-temperature solutions:
 structure determination using the traditional 3-D and the 4-D superspace
 group methods and magnetic measurements on oriented single crystals
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              8790
_journal_page_last               8796
_journal_volume                  123
_journal_year                    2001
_chemical_formula_sum            Sr6
_chemical_name_systematic        'Sr6 Rh5 O15'
_space_group_IT_number           165
_symmetry_space_group_name_Hall  '-P 3 2"c'
_symmetry_space_group_name_H-M   'P -3 c 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   9.6517
_cell_length_b                   9.6517
_cell_length_c                   4.3493
_cell_volume                     350.879
_citation_journal_id_ASTM        JACSAT
_cod_data_source_file            Stitzer_JACSAT_2001_1124.cif
_cod_data_source_block           Sr6
_cod_original_cell_volume        350.8792
_cod_database_code               4123971
Europium palladium hydrides
Kohlmann, H.; Yvon, K.; Fischer, H.E.; Inorganic Chemistry 40 (2001) 2608–2613; doi:

data_4343724
_publ_section_title
;
 Europium palladium hydrides
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2608
_journal_page_last               2613
_journal_volume                  40
_journal_year                    2001
_chemical_formula_sum            'D3 Eu Pd'
_chemical_name_systematic        'Eu Pd D3'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.8001
_cell_length_b                   3.8001
_cell_length_c                   3.8001
_cell_volume                     54.876
_citation_journal_id_ASTM        INOCAJ
_cod_data_source_file            Kohlmann_INOCAJ_2001_1074.cif
_cod_data_source_block           D3Eu1Pd1
_cod_original_cell_volume        54.87634
_cod_original_formula_sum        'D3 Eu1 Pd1'
_cod_database_code               4343724
Die Kristallstruktur von Pr Te2
Stoewe, K.; Zeitschrift fuer Anorganische und Allgemeine Chemie 626 (2000) 803–811; doi:

data_1526697
_publ_section_title
;
 Die Kristallstruktur von Pr Te2
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              803
_journal_page_last               811
_journal_volume                  626
_journal_year                    2000
_chemical_formula_sum            'Pr Te2'
_space_group_IT_number           75
_symmetry_space_group_name_Hall  'P 4'
_symmetry_space_group_name_H-M   'P 4'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            16
_cell_length_a                   8.968
_cell_length_b                   8.968
_cell_length_c                   18.119
_cell_volume                     1457.221
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Stoewe_ZAACAB_2000_797.cif
_cod_data_source_block           Pr1Te2
_cod_original_formula_sum        'Pr1 Te2'
_cod_database_code               1526697
High-pressure synthesis of novel europium magnesium hydrides
Kohlmann, H.; Bertheville, B.; Yvon, K.; Hansen, T.; Journal of Alloys Compd. 322 (2001) 59–68; doi:

data_1526698
_publ_section_title
;
 High-pressure synthesis of novel europium magnesium hydrides
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              59
_journal_page_last               68
_journal_volume                  322
_journal_year                    2001
_chemical_formula_sum            'D6 Eu2 Mg'
_chemical_name_systematic        'Eu2 Mg D6'
_space_group_IT_number           164
_symmetry_space_group_name_Hall  '-P 3 2"'
_symmetry_space_group_name_H-M   'P -3 m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   5.50644
_cell_length_b                   5.50644
_cell_length_c                   4.10054
_cell_volume                     107.675
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Kohlmann_JALCEU_2001_1293.cif
_cod_data_source_block           D6Eu2Mg1
_cod_original_cell_volume        107.6747
_cod_original_formula_sum        'D6 Eu2 Mg1'
_cod_database_code               1526698
Possibilities of the Ce Ni2 Si2 hydrogenation under mechanical treatment
Streletskii, A.N.; Morozkin, A.V.; Portnoy, V.K.; Berestetskaya, I.V.; Verbetskii, V.N.; Materials Research Bulletin 35 (2000) 719–726; doi:

data_1526699
_publ_section_title
;
 Possibilities of the Ce Ni2 Si2 hydrogenation under mechanical treatment
;
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              719
_journal_page_last               726
_journal_volume                  35
_journal_year                    2000
_chemical_formula_sum            'Ce Ni2 Si2'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.0259
_cell_length_b                   4.0259
_cell_length_c                   9.556
_cell_volume                     154.882
_citation_journal_id_ASTM        MRBUAC
_cod_data_source_file            Streletskii_MRBUAC_2000_326.cif
_cod_data_source_block           Ce1Ni2Si2
_cod_original_cell_volume        154.8824
_cod_original_formula_sum        'Ce1 Ni2 Si2'
_cod_database_code               1526699
High-pressure synthesis of novel europium magnesium hydrides
Kohlmann, H.; Bertheville, B.; Hansen, T.; Yvon, K.; Journal of Alloys Compd. 322 (2001) 59–68; doi:

data_1526700
_publ_section_title
;
 High-pressure synthesis of novel europium magnesium hydrides
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              59
_journal_page_last               68
_journal_volume                  322
_journal_year                    2001
_chemical_formula_sum            'D26 Eu6 Mg7'
_chemical_name_systematic        'Eu6 Mg7 D26'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-I 2y'
_symmetry_space_group_name_H-M   'I 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.683
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   14.0939
_cell_length_b                   5.6455
_cell_length_c                   11.509
_cell_volume                     915.673
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Kohlmann_JALCEU_2001_1294.cif
_cod_data_source_block           D26Eu6Mg7
_cod_original_cell_volume        915.6729
_cod_original_sg_symbol_Hall     '-C 2y (x,y,-x+z)'
_cod_database_code               1526700
High-pressure synthesis of novel europium magnesium hydrides
Kohlmann, H.; Bertheville, B.; Hansen, T.; Yvon, K.; Journal of Alloys Compd. 322 (2001) 59–68; doi:

data_1526701
_publ_section_title
;
 High-pressure synthesis of novel europium magnesium hydrides
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              59
_journal_page_last               68
_journal_volume                  322
_journal_year                    2001
_chemical_formula_sum            'D10 Eu2 Mg3'
_chemical_name_systematic        'Eu2 Mg3 D10'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 111.478
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   17.4841
_cell_length_b                   5.7231
_cell_length_c                   7.3647
_cell_volume                     685.762
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Kohlmann_JALCEU_2001_1295.cif
_cod_data_source_block           D10Eu2Mg3
_cod_original_cell_volume        685.7617
_cod_database_code               1526701
Low-temperature deuterium ordering in the cubic Laves phase derivative alpha-(Zr Cr2 D0.66)
Kohlmann, H.; Yvon, K.; Fauth, F.; Skripov, A.V.; Fischer, P.; Kozhanov, V.N.; Journal of Alloys Compd. 327 (2001) 4–9; doi:

data_1526702
_publ_section_title
;
 Low-temperature deuterium ordering in the cubic Laves phase derivative
 alpha-(Zr Cr2 D0.66)
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              4
_journal_page_last               9
_journal_volume                  327
_journal_year                    2001
_chemical_formula_sum            'Cr2 D0.66 Zr'
_chemical_name_systematic        'Zr Cr2 D0.66'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   7.2918
_cell_length_b                   7.2918
_cell_length_c                   7.2918
_cell_volume                     387.708
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Kohlmann_JALCEU_2001_1327.cif
_cod_data_source_block           D0.66Cr2Zr1
_cod_original_cell_volume        387.7076
_cod_original_formula_sum        'D0.66 Cr2 Zr1'
_cod_database_code               1526702
Crystal structure of a new monophosphate tungsten(V) bronze with hexagonal tunnels Na4 (W O3)8 (P O2)4
Stus', N.V.; Lisnyak, V.V.; Slobodyanik, N.S.; Journal of Alloys Compd. 325 (2001) 73–77; doi:

data_1526703
_publ_section_title
;
 Crystal structure of a new monophosphate tungsten(V) bronze with
 hexagonal tunnels Na4 (W O3)8 (P O2)4
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              73
_journal_page_last               77
_journal_volume                  325
_journal_year                    2001
_chemical_formula_sum            'Na O8 P W2'
_chemical_name_systematic        'Na ((W O3)2 (P O2))'
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 99.5898
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   6.6065
_cell_length_b                   5.2711
_cell_length_c                   8.8898
_cell_volume                     305.248
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Stus_JALCEU_2001_1315.cif
_cod_data_source_block           Na1O8P1W2
_cod_original_cell_volume        305.2481
_cod_original_formula_sum        'Na1 O8 P1 W2'
_cod_database_code               1526703
Low-temperature deuterium ordering in the cubic Laves phase derivative alpha-(Zr Cr2 D0.66)
Kohlmann, H.; Skripov, A.V.; Fauth, F.; Fischer, P.; Yvon, K.; Kozhanov, V.N.; Journal of Alloys Compd. 327 (2001) 4–9; doi:

data_1526704
_publ_section_title
;
 Low-temperature deuterium ordering in the cubic Laves phase derivative
 alpha-(Zr Cr2 D0.66)
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              4
_journal_page_last               9
_journal_volume                  327
_journal_year                    2001
_chemical_formula_sum            'Cr2 D0.61 Zr'
_chemical_name_systematic        'Zr Cr2 D0.61'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 109.563
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.9411
_cell_length_b                   5.1372
_cell_length_c                   8.905
_cell_volume                     385.415
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Kohlmann_JALCEU_2001_1328.cif
_cod_data_source_block           D0.61Cr2Zr1
_cod_original_cell_volume        385.4149
_cod_original_sg_symbol_Hall     '-P 2ybc (x-z,y,z)'
_cod_original_formula_sum        'D0.61 Cr2 Zr1'
_cod_database_code               1526704
Structural studies of the superconducting La2.5 Y0.5 Ca Ba3 (Cu1-x Fex)7 Oz 8 (0 <= x <= 0.1) perovskite system by neutron diffraction
Subbarao, M.V.; Kundaliya, D.C.; Yelon, W.B.; Kulkarni, R.G.; Malik, S.K.; Journal of Superconductivity 14 (2001) 397–403; doi:

data_1526705
_publ_section_title
;
 Structural studies of the superconducting La2.5 Y0.5 Ca Ba3 (Cu1-x Fex)7
 Oz 8 (0 <= x <= 0.1) perovskite system by neutron diffraction
;
_journal_name_full               'Journal of Superconductivity'
_journal_page_first              397
_journal_page_last               403
_journal_volume                  14
_journal_year                    2001
_chemical_formula_sum
'Ba1.286 Ca0.429 Cu2.886 Fe0.114 La1.071 O7.032 Y0.214'
_chemical_name_systematic
;
(La0.357 Y0.214 Ca0.429) (Ba0.643 La0.357)2 Cu (Cu1.886 Fe0.114) O7.032
;
_space_group_IT_number           123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.869
_cell_length_b                   3.869
_cell_length_c                   11.6697
_cell_volume                     174.686
_citation_journal_id_ASTM        JOUSEH
_cod_data_source_file            Subbarao_JOUSEH_2001_1429.cif
_cod_data_source_block           Ba1.286Ca0.429Cu2.886Fe0.114La1.071O7.032Y0.214
_cod_original_cell_volume        174.6856
_cod_database_code               1526705
Crystal structure of (N H4)2 Sn2 F4 (N O3)2 - first example of dimer complexes (Sn2 F4 E2) in tin(II) fluorides
Kokunov, Yu.V.; Detkov, D.G.; Gorbunova, Yu.E.; Ershova, M.M.; Buslaev, Yu.A.; Mikhailov, Yu.N.; Doklady Akad. Nauk 378 (2001) 347–350; doi:

data_1526706
_publ_section_title
;
 Crystal structure of (N H4)2 Sn2 F4 (N O3)2 - first example of dimer
 complexes (Sn2 F4 E2) in tin(II) fluorides
;
_journal_name_full               'Doklady Akad. Nauk'
_journal_page_first              347
_journal_page_last               350
_journal_volume                  378
_journal_year                    2001
_chemical_formula_sum            'F4 H8 N4 O6 Sn2'
_chemical_name_systematic        '(N H4)2 (Sn2 F4 (N O3)2)'
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'C 2y'
_symmetry_space_group_name_H-M   'C 1 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 110.47
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   14.897
_cell_length_b                   5.412
_cell_length_c                   7.167
_cell_volume                     541.336
_citation_journal_id_ASTM        DAKNEQ
_cod_data_source_file            Kokunov_DAKNEQ_2001_1039.cif
_cod_data_source_block           H8F4N4O6Sn2
_cod_original_cell_volume        541.3356
_cod_original_formula_sum        'H8 F4 N4 O6 Sn2'
_cod_database_code               1526706
Structural studies of the superconducting La2.5 Y0.5 Ca Ba3 (Cu1-x Fex)7 Oz 8 (0 <= x <= 0.1) perovskite system by neutron diffraction
Subbarao, M.V.; Kundaliya, D.C.; Kulkarni, R.G.; Malik, S.K.; Yelon, W.B.; Journal of Superconductivity 14 (2001) 397–403; doi:

data_1526707
_publ_section_title
;
 Structural studies of the superconducting La2.5 Y0.5 Ca Ba3 (Cu1-x Fex)7
 Oz 8 (0 <= x <= 0.1) perovskite system by neutron diffraction
;
_journal_name_full               'Journal of Superconductivity'
_journal_page_first              397
_journal_page_last               403
_journal_volume                  14
_journal_year                    2001
_chemical_formula_sum
'Ba1.286 Ca0.429 Cu2.764 Fe0.236 La1.071 O7.24 Y0.214'
_chemical_name_systematic
;
(La0.357 Y0.214 Ca0.429) (Ba0.643 La0.357)2 Cu (Cu1.764 Fe0.236) O7.24
;
_space_group_IT_number           123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.8707
_cell_length_b                   3.8707
_cell_length_c                   11.6225
_cell_volume                     174.132
_citation_journal_id_ASTM        JOUSEH
_cod_data_source_file            Subbarao_JOUSEH_2001_1430.cif
_cod_data_source_block           Ba1.286Ca0.429Cu2.764Fe0.236La1.071O7.24Y0.214
_cod_database_code               1526707
Synthesis and crystal structure of calcium trifluorostannate(II)
Kokunov, Yu.V.; Detkov, D.G.; Ershova, M.M.; Gorbunova, Yu.E.; Mikhailov, Yu.N.; Doklady Akad. Nauk 376 (2001) 635–637; doi:

data_1526708
_publ_section_title
;
 Synthesis and crystal structure of calcium trifluorostannate(II)
;
_journal_name_full               'Doklady Akad. Nauk'
_journal_page_first              635
_journal_page_last               637
_journal_volume                  376
_journal_year                    2001
_chemical_formula_sum            'Ca F6 Sn2'
_chemical_name_systematic        'Ca (Sn F3)2'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                98.72
_cell_angle_beta                 101.94
_cell_angle_gamma                92.65
_cell_formula_units_Z            2
_cell_length_a                   4.419
_cell_length_b                   7.191
_cell_length_c                   9.834
_cell_volume                     301.226
_citation_journal_id_ASTM        DAKNEQ
_cod_data_source_file            Kokunov_DAKNEQ_2001_990.cif
_cod_data_source_block           Ca1F6Sn2
_cod_original_cell_volume        301.2259
_cod_original_formula_sum        'Ca1 F6 Sn2'
_cod_database_code               1526708
Structural studies of the superconducting La2.5 Y0.5 Ca Ba3 (Cu1-x Fex)7 Oz 8 (0 <= x <= 0.1) perovskite system by neutron diffraction
Subbarao, M.V.; Kundaliya, D.C.; Kulkarni, R.G.; Malik, S.K.; Yelon, W.B.; Journal of Superconductivity 14 (2001) 397–403; doi:

data_1526709
_publ_section_title
;
 Structural studies of the superconducting La2.5 Y0.5 Ca Ba3 (Cu1-x Fex)7
 Oz 8 (0 <= x <= 0.1) perovskite system by neutron diffraction
;
_journal_name_full               'Journal of Superconductivity'
_journal_page_first              397
_journal_page_last               403
_journal_volume                  14
_journal_year                    2001
_chemical_formula_sum
'Ba1.286 Ca0.429 Cu2.698 Fe0.302 La1.071 O7.292 Y0.214'
_chemical_name_systematic
;
(La0.357 Y0.214 Ca0.429) (Ba0.643 La0.357)2 Cu (Cu1.698 Fe0.302) O7.292
;
_space_group_IT_number           123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.8772
_cell_length_b                   3.8772
_cell_length_c                   11.6318
_cell_volume                     174.857
_citation_journal_id_ASTM        JOUSEH
_cod_data_source_file            Subbarao_JOUSEH_2001_1431.cif
_cod_data_source_block           Ba1.286Ca0.429Cu2.698Fe0.302La1.071O7.292Y0.214
_cod_original_cell_volume        174.8571
_cod_database_code               1526709
Magnetic structures of R T Sb2 (R = Pr, Nd; T = Cu, Pd) compounds
Kolenda, M.; Leciejewicz, J.; Hofmann, M.; Penc, B.; Zygmunt, A.; Szytula, A.; Journal of Alloys Compd. 315 (2001) 22–27; doi:

data_1526710
_publ_section_title
;
 Magnetic structures of R T Sb2 (R = Pr, Nd; T = Cu, Pd) compounds
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              22
_journal_page_last               27
_journal_volume                  315
_journal_year                    2001
_chemical_formula_sum            'Cu Pr Sb2'
_chemical_name_systematic        'Pr Cu Sb2'
_space_group_IT_number           129
_symmetry_space_group_name_Hall  '-P 4a 2a'
_symmetry_space_group_name_H-M   'P 4/n m m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.3056
_cell_length_b                   4.3056
_cell_length_c                   10.164
_cell_volume                     188.422
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Kolenda_JALCEU_2001_1147.cif
_cod_data_source_block           Cu1Pr1Sb2
_cod_original_cell_volume        188.4222
_cod_original_formula_sum        'Cu1 Pr1 Sb2'
_cod_database_code               1526710
New (Ru (N H3)6) M F6 phases: precursors to catalysts for halogenation reactions
Subramanian, M.A.; Harlow, R.H.; Rao, V.N.M.; Materials Research Bulletin 35 (2000) 1587–1592; doi:

data_1526711
_publ_section_title
;
 New (Ru (N H3)6) M F6 phases: precursors to catalysts for halogenation
 reactions
;
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              1587
_journal_page_last               1592
_journal_volume                  35
_journal_year                    2000
_chemical_formula_sum            'Al F6 H18 N6 Ru'
_chemical_name_systematic        '(Ru (N H3)6) (Al F6)'
_space_group_IT_number           205
_symmetry_space_group_name_Hall  '-P 2ac 2ab 3'
_symmetry_space_group_name_H-M   'P a -3'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.9872
_cell_length_b                   9.9872
_cell_length_c                   9.9872
_cell_volume                     996.165
_citation_journal_id_ASTM        MRBUAC
_cod_data_source_file            Subramanian_MRBUAC_2000_296.cif
_cod_data_source_block           H18Al1F6N6Ru1
_cod_original_cell_volume        996.1649
_cod_original_formula_sum        'H18 Al1 F6 N6 Ru1'
_cod_database_code               1526711
Magnetic structures of R T Sb2 (R = Pr, Nd; T = Cu, Pd) compounds
Kolenda, M.; Penc, B.; Hofmann, M.; Leciejewicz, J.; Zygmunt, A.; Szytula, A.; Journal of Alloys Compd. 315 (2001) 22–27; doi:

data_1526712
_publ_section_title
;
 Magnetic structures of R T Sb2 (R = Pr, Nd; T = Cu, Pd) compounds
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              22
_journal_page_last               27
_journal_volume                  315
_journal_year                    2001
_chemical_formula_sum            'Pd Pr Sb2'
_chemical_name_systematic        'Pr Pd Sb2'
_space_group_IT_number           129
_symmetry_space_group_name_Hall  '-P 4a 2a'
_symmetry_space_group_name_H-M   'P 4/n m m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.4759
_cell_length_b                   4.4759
_cell_length_c                   9.8182
_cell_volume                     196.695
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Kolenda_JALCEU_2001_1148.cif
_cod_data_source_block           Pd1Pr1Sb2
_cod_original_cell_volume        196.6947
_cod_original_formula_sum        'Pd1 Pr1 Sb2'
_cod_database_code               1526712